| ||Format||Pages||Price|| |
|6||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||12||$62.00||  ADD TO CART|
Significance and Use
5.1 Several physical properties of rigid cellular plastics are dependent on cell size and cell orientation. Measuring water absorption and open-cell content in accordance with Test Method and Test Method requires knowledge of surface cell volume, which uses cell size values in the calculations.
5.2 This test method provides an apparent cell size because it assumes that there is no measurable edge to edge or top to bottom variation in average cell size and that the cell size distribution about the average cell size is normal. If the analyst is concerned there may be significant variation in either the average cell size or the cell size distribution more detailed analysis may be required.
5.3 Before proceeding with this test method, reference should be made to the specification of the material being tested. Any test specimen preparation, conditioning, dimensions, or testing parameters, or a combination thereof, covered in the materials specification shall take precedence over those mentioned in this test method. If there are no material specifications, then the default conditions apply.
FIG. 1 Razor Blade Cell Size Specimen Slicer
FIG. 2 Cell Size Scale Slide Assembly
1.1 This test method covers the determination of the apparent cell size of rigid cellular plastics by counting the number of cell-wall intersections in a specified distance.
1.2 Procedure A requires the preparation of a thin slice, not more than one half the average cell diameter in thickness, that is mechanically stable. For most rigid cellular plastics this limits the test method to materials with an average cell size of at least 0.2 mm.
1.3 Procedure B is intended for use with materials whose friable nature makes it difficult to obtain a thin slice for viewing.
1.4 The values stated in SI units are to be regarded as standard. The values given in parentheses are for information only.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
Note 1: The annex to ISO 2896 is technically equivalent to this test method.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D883 Terminology Relating to Plastics
D2842 Test Method for Water Absorption of Rigid Cellular Plastics
D6226 Test Method for Open Cell Content of Rigid Cellular Plastics
E456 Terminology Relating to Quality and Statistics
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
ISO StandardISO 2896 Cellular Plastics, RigidDetermination of Water Absorption Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org.
ICS Number Code 83.100 (Cellular materials)
UNSPSC Code 13111300(Foams)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D3576-20, Standard Test Method for Cell Size of Rigid Cellular Plastics, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top